#------------------------------------------------------------------------------
#$Date: 2016-02-13 21:28:24 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176429 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/26/4002607.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4002607
loop_
_publ_author_name
'Ishizawa, Nobuo'
'Asaka, Toru'
'Kudo, Tatsunari'
'Fukuda, Koichiro'
'Yasuhara, Akira'
'Abe, Nobuyuki'
'Arima, Taka-hisa'
_publ_section_title
;
 Structural Evolution of GdBaCo2O5+δ(δ = 7/18) at Elevated Temperatures
;
_journal_name_full               'Chemistry of Materials'
_journal_page_first              141114094038007
_journal_paper_doi               10.1021/cm503132e
_journal_year                    2014
_chemical_formula_sum            'Ba Co2 Gd O5.389'
_chemical_formula_weight         498.7
_chemical_name_systematic        ' ?'
_space_group_IT_number           47
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.8734(5)
_cell_length_b                   7.8344(8)
_cell_length_c                   7.5592(10)
_cell_measurement_temperature    399
_cell_volume                     229.39(5)
_diffrn_ambient_temperature      399
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0786
_diffrn_reflns_av_sigmaI/netI    0.0295
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            1245
_diffrn_reflns_theta_full        30.01
_diffrn_reflns_theta_max         30.01
_diffrn_reflns_theta_min         2.6
_exptl_absorpt_coefficient_mu    29.77
_exptl_absorpt_correction_T_max  0.211778
_exptl_absorpt_correction_T_min  0.114412
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 1996)'
_exptl_crystal_density_diffrn    7.2198
_exptl_crystal_description       sphere
_exptl_crystal_F_000             434
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_exptl_crystal_size_rad          0.04
_refine_diff_density_max         2.40
_refine_diff_density_min         -3.36
_refine_ls_extinction_coef       214(19)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    2.34
_refine_ls_goodness_of_fit_ref   2.12
_refine_ls_number_constraints    0
_refine_ls_number_parameters     32
_refine_ls_number_reflns         770
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0496
_refine_ls_R_factor_gt           0.0442
_refine_ls_shift/su_max          0.0027
_refine_ls_shift/su_mean         0.0010
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0543
_refine_ls_wR_factor_ref         0.0550
_reflns_number_gt                617
_reflns_number_total             770
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            cm503132e_si_002.cif
_cod_data_source_block           125c
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to /home/saulius/struct/CIF-dictionaries/IUCr/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.5 from 2014-11-21.

Automatic conversion script
Id: cif_fix_values 3866 2015-08-17 15:13:47Z robertas 
;
_cod_original_sg_symbol_Hall     '-P -2x;-2y;-2z'
_cod_original_formula_sum        'Ba1 Co2 Gd1 O5.389'
_cod_database_code               4002607
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 -x,-y,-z
6 x,y,-z
7 x,-y,z
8 -x,y,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
Ba1 Ba 0 0.25102(8) 0 Uani 0.0099(4) 2 1 d
Gd1 Gd 0 0.2364(2) 0.5 Uani 0.0127(4) 2 1 d
Co1a Co 0.5 0 0.25243(19) Uani 0.0076(9) 2 1 d
Co1b Co 0.5 0.5 0.25521(19) Uani 0.0084(9) 2 1 d
O1a O 0.5 0.5 0 Uiso 0.014(3) 1 1 d
O1b O 0.5 0 0 Uiso 0.014(3) 1 1 d
O2a O 0 0.5 0.303(2) Uiso 0.016(3) 2 1 d
O2b O 0 0 0.278(2) Uiso 0.016(3) 2 1 d
O2c O 0.5 0.2594(8) 0.303(2) Uiso 0.020(3) 4 1 d
O3 O 0.5 0 0.5 Uiso 0.035(5) 1 0.7778 d
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba -0.3244 2.2819 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Co 0.3494 0.9721 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Gd -0.1653 3.9035 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1a Ba1 O1a 1_455 . 89.59(2)
O1a Ba1 O1b 1_455 1_455 90.644(9)
O1a Ba1 O1b 1_455 . 179.766(19)
O1a Ba1 O2a 1_455 . 62.59(13)
O1a Ba1 O2a 1_455 3_555 62.59(13)
O1a Ba1 O2b 1_455 . 118.98(12)
O1a Ba1 O2b 1_455 3_555 118.98(12)
O1a Ba1 O2c 1_455 1_455 61.93(16)
O1a Ba1 O2c 1_455 . 116.06(15)
O1a Ba1 O2c 1_455 3_555 61.93(16)
O1a Ba1 O2c 1_455 3_655 116.06(15)
O1a Ba1 O1b . 1_455 179.766(19)
O1a Ba1 O1b . . 90.644(9)
O1a Ba1 O2a . . 62.59(13)
O1a Ba1 O2a . 3_555 62.59(13)
O1a Ba1 O2b . . 118.98(12)
O1a Ba1 O2b . 3_555 118.98(12)
O1a Ba1 O2c . 1_455 116.06(15)
O1a Ba1 O2c . . 61.93(16)
O1a Ba1 O2c . 3_555 116.06(15)
O1a Ba1 O2c . 3_655 61.93(16)
O1b Ba1 O1b 1_455 . 89.12(2)
O1b Ba1 O2a 1_455 . 117.53(13)
O1b Ba1 O2a 1_455 3_555 117.53(13)
O1b Ba1 O2b 1_455 . 60.89(12)
O1b Ba1 O2b 1_455 3_555 60.89(12)
O1b Ba1 O2c 1_455 1_455 64.06(15)
O1b Ba1 O2c 1_455 . 117.95(16)
O1b Ba1 O2c 1_455 3_555 64.06(15)
O1b Ba1 O2c 1_455 3_655 117.95(16)
O1b Ba1 O2a . . 117.53(13)
O1b Ba1 O2a . 3_555 117.53(13)
O1b Ba1 O2b . . 60.89(12)
O1b Ba1 O2b . 3_555 60.89(12)
O1b Ba1 O2c . 1_455 117.95(16)
O1b Ba1 O2c . . 64.06(15)
O1b Ba1 O2c . 3_555 117.95(16)
O1b Ba1 O2c . 3_655 64.06(15)
O2a Ba1 O2a . 3_555 99.1(3)
O2a Ba1 O2b . . 83.5(3)
O2a Ba1 O2b . 3_555 177.4(3)
O2a Ba1 O2c . 1_455 53.5(2)
O2a Ba1 O2c . . 53.5(2)
O2a Ba1 O2c . 3_555 124.5(2)
O2a Ba1 O2c . 3_655 124.5(2)
O2a Ba1 O2b 3_555 . 177.4(3)
O2a Ba1 O2b 3_555 3_555 83.5(3)
O2a Ba1 O2c 3_555 1_455 124.5(2)
O2a Ba1 O2c 3_555 . 124.5(2)
O2a Ba1 O2c 3_555 3_555 53.5(2)
O2a Ba1 O2c 3_555 3_655 53.5(2)
O2b Ba1 O2b . 3_555 93.9(3)
O2b Ba1 O2c . 1_455 57.1(2)
O2b Ba1 O2c . . 57.1(2)
O2b Ba1 O2c . 3_555 124.9(2)
O2b Ba1 O2c . 3_655 124.9(2)
O2b Ba1 O2c 3_555 1_455 124.9(2)
O2b Ba1 O2c 3_555 . 124.9(2)
O2b Ba1 O2c 3_555 3_555 57.1(2)
O2b Ba1 O2c 3_555 3_655 57.1(2)
O2c Ba1 O2c 1_455 . 80.4(3)
O2c Ba1 O2c 1_455 3_555 99.5(3)
O2c Ba1 O2c 1_455 3_655 177.49(18)
O2c Ba1 O2c . 3_555 177.49(18)
O2c Ba1 O2c . 3_655 99.5(3)
O2c Ba1 O2c 3_555 3_655 80.4(3)
O2a Gd1 O2a . 3_556 71.7(5)
O2a Gd1 O2b . . 102.0(4)
O2a Gd1 O2b . 3_556 173.7(4)
O2a Gd1 O2c . 1_455 65.4(2)
O2a Gd1 O2c . . 65.4(2)
O2a Gd1 O2c . 3_556 107.3(3)
O2a Gd1 O2c . 3_656 107.3(3)
O2a Gd1 O3 . 1_455 124.07(16)
O2a Gd1 O3 . . 124.07(16)
O2a Gd1 O2b 3_556 . 173.7(4)
O2a Gd1 O2b 3_556 3_556 102.0(4)
O2a Gd1 O2c 3_556 1_455 107.3(3)
O2a Gd1 O2c 3_556 . 107.3(3)
O2a Gd1 O2c 3_556 3_556 65.4(2)
O2a Gd1 O2c 3_556 3_656 65.4(2)
O2a Gd1 O3 3_556 1_455 124.07(16)
O2a Gd1 O3 3_556 . 124.07(16)
O2b Gd1 O2b . 3_556 84.3(4)
O2b Gd1 O2c . 1_455 69.3(3)
O2b Gd1 O2c . . 69.3(3)
O2b Gd1 O2c . 3_556 117.5(2)
O2b Gd1 O2c . 3_656 117.5(2)
O2b Gd1 O3 . 1_455 59.16(14)
O2b Gd1 O3 . . 59.16(14)
O2b Gd1 O2c 3_556 1_455 117.5(2)
O2b Gd1 O2c 3_556 . 117.5(2)
O2b Gd1 O2c 3_556 3_556 69.3(3)
O2b Gd1 O2c 3_556 3_656 69.3(3)
O2b Gd1 O3 3_556 1_455 59.16(14)
O2b Gd1 O3 3_556 . 59.16(14)
O2c Gd1 O2c 1_455 . 104.4(4)
O2c Gd1 O2c 1_455 3_556 74.9(4)
O2c Gd1 O2c 1_455 3_656 171.6(2)
O2c Gd1 O3 1_455 1_455 58.64(19)
O2c Gd1 O3 1_455 . 128.5(2)
O2c Gd1 O2c . 3_556 171.6(2)
O2c Gd1 O2c . 3_656 74.9(4)
O2c Gd1 O3 . 1_455 128.5(2)
O2c Gd1 O3 . . 58.64(19)
O2c Gd1 O2c 3_556 3_656 104.4(4)
O2c Gd1 O3 3_556 1_455 58.64(19)
O2c Gd1 O3 3_556 . 128.5(2)
O2c Gd1 O3 3_656 1_455 128.5(2)
O2c Gd1 O3 3_656 . 58.64(19)
O3 Gd1 O3 1_455 . 92.55(6)
O1b Co1a O2b . . 95.8(4)
O1b Co1a O2b . 1_655 95.8(4)
O1b Co1a O2c . . 100.6(4)
O1b Co1a O2c . 2_655 100.6(4)
O1b Co1a O3 . . 180.0(5)
O2b Co1a O2b . 1_655 168.5(6)
O2b Co1a O2c . . 88.94(9)
O2b Co1a O2c . 2_655 88.94(9)
O2b Co1a O3 . . 84.2(4)
O2b Co1a O2c 1_655 . 88.94(9)
O2b Co1a O2c 1_655 2_655 88.94(9)
O2b Co1a O3 1_655 . 84.2(4)
O2c Co1a O2c . 2_655 158.7(6)
O2c Co1a O3 . . 79.4(4)
O2c Co1a O3 2_655 . 79.4(4)
O1a Co1b O2a . . 100.5(5)
O1a Co1b O2a . 1_655 100.5(5)
O1a Co1b O2c . . 100.8(5)
O1a Co1b O2c . 2_665 100.8(5)
O2a Co1b O2a . 1_655 159.0(7)
O2a Co1b O2c . . 88.04(13)
O2a Co1b O2c . 2_665 88.04(13)
O2a Co1b O2c 1_655 . 88.04(13)
O2a Co1b O2c 1_655 2_665 88.04(13)
O2c Co1b O2c . 2_665 158.4(7)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Ba1 O1a 1_455 2.7488(6)
Ba1 O1a . 2.7488(6)
Ba1 O1b 1_455 2.7601(6)
Ba1 O1b . 2.7601(6)
Ba1 O2a . 3.006(13)
Ba1 O2a 3_555 3.006(13)
Ba1 O2b . 2.880(11)
Ba1 O2b 3_555 2.880(11)
Ba1 O2c 1_455 2.999(12)
Ba1 O2c . 2.999(12)
Ba1 O2c 3_555 2.999(12)
Ba1 O2c 3_655 2.999(12)
Gd1 O2a . 2.547(10)
Gd1 O2a 3_556 2.547(10)
Gd1 O2b . 2.498(10)
Gd1 O2b 3_556 2.498(10)
Gd1 O2c 1_455 2.450(10)
Gd1 O2c . 2.450(10)
Gd1 O2c 3_556 2.450(10)
Gd1 O2c 3_656 2.450(10)
Gd1 O3 1_455 2.6799(13)
Gd1 O3 . 2.6799(13)
Co1a O1b . 1.9082(15)
Co1a O2b . 1.9466(16)
Co1a O2b 1_655 1.9466(16)
Co1a O2c . 2.068(7)
Co1a O2c 2_655 2.068(7)
Co1a O3 . 1.8714(15)
Co1b O1a . 1.9292(15)
Co1b O2a . 1.970(3)
Co1b O2a 1_655 1.970(3)
Co1b O2c . 1.919(7)
Co1b O2c 2_665 1.919(7)
#BEGIN Loops that were not found in dictionaries:
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.536(12) 1 0 0 0 1 0 0 0 1
2 0.464(12) 0.015 -2.0274 -0.0001 0.4931 0.015 0.001 -0.0005 -0.0001 1
loop_
_jana_atom_site_adp_c_label
_jana_atom_site_adp_c_type_symbol
_jana_atom_site_adp_c_111
_jana_atom_site_adp_c_112
_jana_atom_site_adp_c_113
_jana_atom_site_adp_c_122
_jana_atom_site_adp_c_123
_jana_atom_site_adp_c_133
_jana_atom_site_adp_c_222
_jana_atom_site_adp_c_223
_jana_atom_site_adp_c_233
_jana_atom_site_adp_c_333
Gd1 Gd 0 0.0011(14) 0 0 0 0 0.0005(6) 0 -0.0002(3) 0
#END Loops that were not found in dictionaries
